| ||Format||Pages||Price|| |
|PDF Version||16||$48.00||  ADD TO CART|
|Print Version||16||$48.00||  ADD TO CART|
|Standard + Redline PDF Bundle||32||$57.60||  ADD TO CART|
This specification covers seamless wrought zirconium-alloy tubes for nuclear reactor fuel cladding application. Two grades of reactor grade zirconium alloys are described. Tubes covered by this specification shall be made from ingots produced by multiple vacuum arc or electron beam melting in furnaces of a type conventionally used for reactive materials. The tubes shall conform to the requirements for chemical composition prescribed. Recrsytallisation annealed tubes shall conform to the requirements for mechanical properties at room temperature prescribed. The tension test shall be conducted. Yield strength and tension properties shall be determined. Burst testing, when specified, shall be performed at room temperature on finished tubing.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers seamless wrought zirconium-alloy tubes for nuclear fuel cladding application, in the outside diameter (OD) size range of 0.200 in. (5.1 mm) to 0.650 in. (16.5 mm) and wall thickness range of 0.010 in. (0.25 mm) to 0.035 in. (0.89 mm).
1.2.1 The present UNS numbers designated for the two grades are given in Table 1.
1.3 Unless a single unit is used, for example corrosion mass gain in mg/dm2, the values stated in either inch-pound or SI units are to be regarded separately as standard. The values stated in each system are not exact equivalents; therefore each system must be used independently of the other. SI values cannot be mixed with inch-pound values.
1.4 The following precautionary caveat pertains only to the test method portions of this specification: This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B350/B350M Specification for Zirconium and Zirconium Alloy Ingots for Nuclear Application
B353 Specification for Wrought Zirconium and Zirconium Alloy Seamless and Welded Tubes for Nuclear Service (Except Nuclear Fuel Cladding)
E8 Test Methods for Tension Testing of Metallic Materials
E8M Test Methods for Tension Testing of Metallic Materials [Metric]
E21 Test Methods for Elevated Temperature Tension Tests of Metallic Materials
E29 Practice for Using Significant Digits in Test Data to Determine Conformance with Specifications
E112 Test Methods for Determining Average Grain Size
G2/G2M Test Method for Corrosion Testing of Products of Zirconium, Hafnium, and Their Alloys in Water at 680F [360C] or in Steam at 750F [400C]
Other DocumentANSIB46.1 Surface Texture (Surface Roughness) Available from American Iron and Steel Institute (AISI), 1140 Connecticut Ave., NW, Suite 705, Washington, DC 20036, http://www.steel.org.
ICS Number Code 23.040.15 (Non-ferrous metal pipes)
UNSPSC Code 40180000(Tubes tubing and tube fittings); 26142201(Nuclear fuel cladding tubes)